Ambiguities in the structure determination of antimony tellurides arising from almost homometric structure models and stacking disorder
Schneider, Matthias N.; Seibald, Markus; Lagally, Patrick; Oeckler, Oliver; Journal of Applied Crystallography 43 (2010) 1012–1020; doi:10.1107/S0021889810032644

data_2300299
_publ_section_title
;
 Ambiguities in the structure determination of antimony tellurides arising
 from almost homometric structure models and stacking disorder
;
_journal_coden_ASTM              JACGAR
_journal_coeditor_code           DB5086
_journal_issue                   5
_journal_name_full               'Journal of Applied Crystallography'
_journal_page_first              1012
_journal_page_last               1020
_journal_paper_doi               10.1107/S0021889810032644
_journal_volume                  43
_journal_year                    2010
_chemical_formula_sum            'Sb10 Te3'
_chemical_formula_weight         1600.30
_chemical_name_common            'decaantimony tritelluride'
_chemical_name_systematic
;
 decaantimony tritelluride
;
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   none
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   4.2890(10)
_cell_length_b                   4.2890(10)
_cell_length_c                   75.51(2)
_cell_measurement_reflns_used    1040
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      24
_cell_measurement_theta_min      4
_cell_volume                     1202.9(5)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.982
_diffrn_measured_fraction_theta_max 0.982
_diffrn_measurement_device_type  'Stoe IPDS'
_diffrn_measurement_method       oscillation
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0965
_diffrn_reflns_av_sigmaI/netI    0.0472
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       89
_diffrn_reflns_limit_l_min       -93
_diffrn_reflns_number            2811
_diffrn_reflns_theta_full        25.99
_diffrn_reflns_theta_max         25.99
_diffrn_reflns_theta_min         2.43
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    21.866
_exptl_absorpt_correction_T_max  0.989
_exptl_absorpt_correction_T_min  0.269
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Progam XPREP, from equivalents'
_exptl_crystal_colour            metallic_dark_grey
_exptl_crystal_density_diffrn    6.627
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'irregular polyhedron'
_exptl_crystal_F_000             1998
_exptl_crystal_size_max          0.08
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.01
_refine_diff_density_max         3.189
_refine_diff_density_min         -3.554
_refine_ls_extinction_coef       0.00057(7)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.707
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     22
_refine_ls_number_reflns         375
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.707
_refine_ls_R_factor_all          0.1015
_refine_ls_R_factor_gt           0.0615
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0100P)^2^+5.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1128
_refine_ls_wR_factor_ref         0.1228
_reflns_number_gt                195
_reflns_number_total             375
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            db5086.cif
_cod_data_source_block           hr
_cod_original_sg_symbol_Hall     '-R 3 2" '
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_database_code               2300299